Introduction to the_high_temperature_oxidation_of_metals
This page intentionally left blank
I N T RO DUCT ION TO THE HI GH- TEMP ERATURE OXIDATION OF METALSA straightfoward treatment describing the oxidation processes of metals and alloysat elevated temperatures. This new edition retains the fundamental theory but incor-porates advances made in understanding degradation phenomena. Oxidation pro-cesses in complex systems are dicussed, from reactions in mixed environmentsto protective techniques, including coatings and atmosphere control. The authorsprovide a logical and expert treatment of the subject, producing a revised bookthat will be of use to students studying degradation of high-temperature materialsand an essential guide to researchers requiring an understanding of this elementaryprocess.neil birks was Professor Emeritus in the Department of Materials Science andEngineering at the University of Pittsburgh.gerald h. meier is William Kepler Whiteford Professor in the Department ofMaterials Science and Engineering at the University of Pittsburgh.fred s. pettit is Harry S. Tack Professor in the Department of Materials Scienceand Engineering at the University of Pittsburgh.
IN TRODUCTI O N TO T HEHIGH-TEM P ERATUR E OXIDAT ION OF M ETAL S 2nd Edition NEIL BIRKS Formerly of University of Pittsburgh GERALD H. MEIER University of Pittsburgh FRED S. PETTIT University of Pittsburgh
Professor Neil BirksThis book is dedicated to one of its coauthors, Professor Neil Birks, who passedaway during the preparation of the second edition. Neil was an accomplishedresearcher and educator in a number of ﬁelds including high-temperature oxidation,corrosion, erosion, and process metallurgy. He was also a good friend. Neil’s legacy to science and engineering is well established in his scholarlypublications and the numerous students he mentored. It is our hope that this bookwill complete that legacy. GHM FSP
Contents Acknowledgements page viii Preface ix Introduction xi 1 Methods of investigation 1 2 Thermodynamic fundamentals 16 3 Mechanisms of oxidation 39 4 Oxidation of pure metals 75 5 Oxidation of alloys 101 6 Oxidation in oxidants other than oxygen 163 7 Reactions of metals in mixed environments 176 8 Hot corrosion 205 9 Erosion–corrosion of metals in oxidizing atmospheres 25310 Protective coatings 27111 Atmosphere control for the protection of metals during production processes 306 Appendix A. Solution to Fick’s second law for a semi-inﬁnite solid 323 Appendix B. Rigorous derivation of the kinetics of internal oxidation 327 Appendix C. Effects of impurities on oxide defect structures 332 Index 336 vii
AcknowledgementsThe authors gratefully acknowledge the scientiﬁc contributions of former and cur-rent students. Drs. J. M. Rakowski, M. J. Stiger, N. M. Yanar, and M. C. Maris-Sidaare thanked for their assistance in preparing ﬁgures for this book. The authors also greatly appreciate the helpful comments made by Professor J. L.Beuth (Carnegie Mellon University), Professor H. J. Grabke (Max-Planck Instit¨ t uf¨ r Eisenforschung), and Professor R. A. Rapp (Ohio State University) on parts of uthe manuscript. viii
PrefaceFew metals, particularly those in common technological applications, are stablewhen exposed to the atmosphere at both high and low temperatures. Consequently,most metals in service today are subject to deterioration either by corrosion at roomtemperature or by oxidation at high temperature. The degree of corrosion varieswidely. Some metals, such as iron, will rust and oxidize very rapidly whereas othermetals, such as nickel and chromium, are attacked relatively slowly. It will be seenthat the nature of the surface layers produced on the metal plays a major role in thebehaviour of these materials in aggressive atmospheres. The subject of high-temperature oxidation of metals is capable of extensiveinvestigation and theoretical treatment. It is normally found to be a very satisfyingsubject to study. The theoretical treatment covers a wide range of metallurgical,chemical, and physical principles and can be approached by people of a wide rangeof disciplines who, therefore, complement each other’s efforts. Initially, the subject was studied with the broad aim of preventing the deterio-ration of metals in service, i.e., as a result of exposing the metal to high tempera-tures and oxidizing atmospheres. In recent years, a wealth of mechanistic data hasbecome available. These data cover a broad range of phenomena, e.g., mass transportthrough oxide scales, evaporation of oxide or metallic species, the role of mechan-ical stress in oxidation, growth of scales in complex environments containing morethan one oxidant, and the important relationships between alloy composition andmicrostructure and oxidation. Such information is obtained by applying virtuallyevery physical and chemical investigative technique to the subject. In this book the intention is to introduce the subject of high-temperature oxi-dation of metals to students and to professional engineers whose work demandsfamiliarity with the subject. The emphasis of the book is placed ﬁrmly on supplyingan understanding of the basic, or fundamental, processes involved in oxidation. In order to keep to this objective, there has been no attempt to provide an exhaus-tive, or even extensive, review of the literature. In our opinion this would increase ix
Prefacethe factual content without necessarily improving the understanding of the subjectand would, therefore, increase both the size and price of the book without enhanc-ing its objective as an introduction to the subject. Extensive literature quotation isalready available in books previously published on the subject and in review arti-cles. Similarly the treatment of techniques of investigation has been restricted to alevel that is sufﬁcient for the reader to understand how the subject is studied with-out involving an overabundance of experimental details. Such details are availableelsewhere as indicated. After dealing with the classical situations involving the straightforward oxida-tion of metals and alloys in the ﬁrst ﬁve chapters, the ﬁnal chapters extend thediscussion to reactions in mixed environments, i.e., containing more than one oxi-dant, to reactions involving a condensed phase as in hot corrosion, and the addedcomplications caused by erosive particles. Finally, some typical coatings for high-temperature applications and the use of protective atmospheres during processingare described.Pittsburgh GHM2005 FSP x
IntroductionThe primary purpose of this book is to present an introduction to the fundamentalprinciples that govern the interaction of reactive gaseous environments (usuallycontaining oxygen as a component) and solid materials, usually metals, at hightemperatures. These principles are applicable to a variety of applications, whichcan include those where oxidation is desirable, such as forming a resistive silicalayer on silicon-based semiconductors or removing surface defects from steel slabsduring processing by rapid surface oxidation. However, most applications dealwith situations where reaction of the component with the gaseous atmosphere isundesirable and one tries to minimize the rate at which such reactions occur. The term ‘high-temperature’ requires deﬁnition. In contrast to aqueous corrosion,the temperatures considered in this book will always be high enough that water,when present in the systems, will be present as the vapour rather than the liquid.Moreover, when exposed to oxidizing conditions at temperatures between 100and 500 ◦ C, most metals and alloys form thin corrosion products that grow veryslowly and require transmission electron microscopy for detailed characterization.While some principles discussed in this book may be applicable to thin ﬁlms, ‘hightemperature’ is considered to be 500 ◦ C and above. In designing alloys for use at elevated temperatures, the alloys must not only be asresistant as possible to the effects produced by reaction with oxygen, but resistanceto attack by other oxidants in the environment is also necessary. In addition, theenvironment is not always only a gas since, in practice, the deposition of ash on thealloys is not uncommon. It is, therefore, more realistic in these cases to speak ofthe high-temperature corrosion resistance of materials rather than their oxidationresistance. The rate at which the reactions occur is governed by the nature of the reac-tion product which forms. In the case of materials such as carbon the reactionproduct is gaseous (CO and CO2 ), and does not provide a barrier to continuedreaction. The materials that are designed for high-temperature use are protected by xi
Introductionthe formation of a solid reaction product (usually an oxide) which separates thecomponent and atmosphere. The rate of further reaction is controlled by transportof reactants through this solid layer. The materials designed for use at the high-est temperatures are ones which form the oxides with the slowest transport ratesfor reactants (usually α-Al2 O3 or SiO2 ), i.e., those with the slowest growth rates.However, other materials are often used at lower temperatures if their oxides havegrowth rates which are ‘slow enough’ because they may have better mechanicalproperties (strength, creep resistance), may be easier to fabricate into components(good formability/weldability), or are less expensive. In some cases, the barriers necessary to develop the desired resistance to corro-sion can be formed on structural alloys by appropriate composition modiﬁcation.In many practical applications for structural alloys, however, the required compo-sitional changes are not compatible with the required physical properties of thealloys. In such cases, the necessary compositional modiﬁcations are developedthrough the use of coatings on the surfaces of the structural alloys and the desiredreaction-product barriers are developed on the surfaces of the coatings. A rough hierarchy of common engineering alloys with respect to use temperaturewould include the following.r Low-alloy steels, which form M3 O4 (M = Fe, Cr) surface layers, are used to temperatures of about 500 ◦ C.r Titanium-base alloys, which form TiO2 , are used to about 600 ◦ C.r Ferritic stainless steels, which form Cr2 O3 surface layers, are used to about 650 ◦ C. This temperature limit is based on creep properties rather than oxidation rate.r Austenitic Fe–Ni–Cr alloys, which form Cr2 O3 surface layers and have higher creep strength than ferritic alloys, are used to about 850 ◦ C.r Austenitic Ni–Cr alloys, which form Cr2 O3 surface layers, are used to about 950 ◦ C, which is the upper limit for oxidation protection by chromia formation.r Austenitic Ni–Cr–Al alloys, and aluminide and MCrAlY (M = Ni, Co, or Fe) coatings, which form Al2 O3 surface layers, are used to about 1100 ◦ C.r Applications above 1100 ◦ C require the use of ceramics or refractory metals. The lat- ter alloys oxidize catastrophically and must be coated with a more oxidation-resistant material, which usually forms SiO2 .The exercise of ‘alloy selection’ for a given application takes all of the above factorsinto account. While other properties are mentioned from time to time, the emphasisof this book is on oxidation and corrosion behaviour. xii
1 Methods of investigationThe investigation of high-temperature oxidation takes many forms. Usually oneis interested in the oxidation kinetics. Additionally, one is also interested in thenature of the oxidation process, i.e., the oxidation mechanism. Figure 1.1 is asimple schematic of the cross-section of an oxide formed on the surface of a metalor alloy. Mechanistic studies generally require careful examination of the reactionproducts formed with regard to their composition and morphology and often requireexamination of the metal or alloy substrate as well. Subsequent sections of thischapter will deal with the common techniques for measuring oxidation kineticsand examining reaction-product morphologies. In measuring the kinetics of degradation and characterizing the correspond-ing microstructures questions arise as to the conditions to be used. Test condi-tions should be the same as the application under consideration. Unfortunately, theapplication conditions are often not precisely known and, even when known, canbe extremely difﬁcult to establish as a controlled test. Moreover, true simulationtesting is usually impractical because the desired performance period is generallymuch longer than the length of time for which laboratory testing is feasible. Theanswer to this is accelerated, simulation testing. Accelerated, simulation testing requires knowledge of microstructure and mor-phological changes. All materials used in engineering applications exhibit amicrostructural evolution, beginning during fabrication and ending upon termi-nation of their useful lives. In an accelerated test one must select test conditionsthat cause the microstructures to develop that are representative of the application,but in a much shorter time period. In order to use this approach some knowledgeof the degradation process is necessary. Measurements of reaction kineticsIn the cases of laboratory studies, the experimental technique is basically simple.The specimen is placed in a furnace, controlled at the required temperature, and 1
2 Methods of investigation Oxidizing gas Oxide Alloy Figure 1.1 Schematic diagram of the cross-section of an oxide layer formed on the surface of a metal or alloy.allowed to react for the appropriate time. The specimen is then removed, allowedto cool, and examined. Although this procedure is simple, one drawback is that the start time for the reac-tion cannot be accurately established. Several starting procedures are commonlyused.(1) The specimen may simply be placed in the heated chamber containing the reactive atmosphere.(2) The specimen may be placed in the cold chamber containing the atmosphere and then heated.(3) The specimen may be placed in the cold chamber, which is then evacuated or ﬂushed with inert gas, heated and then, at temperature, the reactive gas is admitted. In all cases the start of the reaction is in doubt either because of the time requiredto heat the specimen or the inevitable formation of thin oxide layers, even in inertgases or under vacuum. This is true especially in the case of more reactive metals,so that when the reaction is started by admitting the reactive gas an oxide layeralready exists. Attempts have been made to overcome this by heating initially in hydrogenwhich is then ﬂushed out by the reactive gas. This also takes a ﬁnite time and thusintroduces uncertainty concerning the start of the reaction. Thin specimens may be used to minimize the time required to heat the specimen.In this case care should be taken that they are not so thin and, therefore, of such lowthermal mass that the heat of reaction, released rapidly during the initial oxidationperiod, causes severe specimen overheating. The uncertainty concerning the start of the reactions usually only affects resultsfor short exposure times up to about ten minutes and becomes less noticeable atlonger times. However, in some cases such as selective oxidation of one element
Measurements of reaction kinetics 3from an alloy, these effects can be quite long-lasting. In practice specimens andprocedures must be designed with these factors in mind. Many early investigations were simply concerned with oxidation rates and notwith oxidation mechanisms. The rate of formation of an oxide in a metal accordingto the reaction (1.1), 2M + O2 = 2MO, (1.1)can be investigated by several methods. The extent of the reaction may be measuredby the following.(1) The amount of metal consumed.(2) The amount of oxygen consumed.(3) The amount of oxide produced. Of these only (2) can be assessed continuously and directly.(1) The amount of metal consumed In practice this may be assessed by observing (a) the weight loss of the specimen or (b) the residual metal thickness. In both cases the specimen must be removed from the furnace, thus interrupting the process.(2) The amount of oxygen consumed This may be assessed by observing either the weight gain or the amount of oxygen used. Both of these methods may be used on a continuous and automatic recording basis.(3) The amount of oxide produced This may be assessed by observing the weight of oxide formed or by measuring the oxide thickness. Of course, in the latter case it is necessary to destroy the specimen, as it is with method (1). Of the above methods, only those involving measurement of weight gain andoxygen consumption give the possibility of obtaining continuous results. Theother methods require destruction of the specimen before the measurement canbe achieved and this has the drawback that, in order to obtain a set of kinetic data,it is necessary to use several specimens. Where the specimen and the methods ofinvestigation are such that continuous results can be obtained, one specimen willgive the complete kinetic record of the reaction. When representing oxidation kinetics, any of the variables mentioned above canbe used, and can be measured as a function of time because, of course, they allresult in an assessment of the extent of reaction. Nowadays it is most general tomeasure the change in mass of a specimen exposed to oxidizing conditions. It is found experimentally that several rate laws can be identiﬁed. The principallaws are (1) linear law, (2) parabolic law, and (3) logarithmic law.
4 Methods of investigation(1) The linear law, for which the rate of reaction is independent of time, is found to refer predominantly to reactions whose rate is controlled by a surface-reaction step or by diffusion through the gas phase.(2) The parabolic law, for which the rate is inversely proportional to the square root of time, is found to be obeyed when diffusion through the scale is the rate-determining process.(3) The logarithmic law is only observed for the formation of very thin ﬁlms of oxide, i.e., between 2 and 4 nm, and is generally associated with low temperatures. Under certain conditions some systems might even show composite kinetics,for instance niobium oxidizing in air at about 1000 ◦ C initially conforms to theparabolic law but later becomes linear, i.e., the rate becomes constant at long times. Discontinuous methods of assessment of reaction kineticsIn this case the specimen is weighed and measured and is then exposed to the con-ditions of high-temperature oxidation for a given time, removed, and reweighed.The oxide scale may also be stripped from the surface of the specimen, which isthen weighed. Assessment of the extent of reaction may be carried out quite sim-ply either by noting the mass gain of the oxidized specimen, which is the massof oxygen taken into the scale, or the mass loss of the stripped specimen, whichis equivalent to the amount of metal taken up in scale formation. Alternatively,the changes in specimen dimensions may be measured. As mentioned before thesetechniques yield only one point per specimen with the disadvantages that (a) manyspecimens are needed to plot fully the kinetics of the reaction, (b) the resultsfrom each specimen may not be equivalent because of experimental variations, and(c) the progress of the reaction between the points is not observed. On the other handthey have the obvious advantage that the techniques, and the apparatus required,are extremely simple. In addition, metallographic information is obtained for eachdata point. Continuous methods of assessmentThese methods fall into two types, those which monitor mass gain and those whichmonitor gas consumption. Mass-gain methodsThe simplest method of continuous monitoring is to use a spring balance. In this casethe specimen is suspended from a sensitive spring whose extension is measured,using a cathetometer, as the specimen mass changes as a result of oxidation, thus
Measurements of reaction kinetics 5 Gas exit tube (may be turned, raised, or lowered) Rigid epoxy resin joint Serrated edge (allows point of suspension to be changed) Pyrex tube Pyrex or silica spiral Cathetometer target Silica or refractory tube with ground joint Tube furnace Silica rod suspension Specimen Thermocouple Gas inlet Figure 1.2 Features of a simple spring balance (for advanced design see ref. 1).giving a semi-continuous monitoring of the reaction. Apparatus suitable for thisis shown diagrammatically in Figure 1.2 which is self-explanatory.1 An importantfeature is the design of the upper suspension point. In Figure 1.2 this is shownas a hollow glass tube which also acts as a gas outlet. The tube can be twisted,raised, or lowered to facilitate accurate placing of the specimen and alignment ofthe spring. A suspension piece is rigidly fastened to the glass tube and providesa serrated horizontal support for the spring whose suspension point may thus beadjusted in the horizontal plane. These reﬁnements are required since alignmentbetween the glass tube containing the spring and the furnace tube is never perfectand it is prudent to provide some means of adjustment of the spring position in orderto ensure accurate placing of the specimen. It would be possible of course to equipa spring balance with a moving transformer, which would enable the mass gain to
6 Methods of investigationbe measured electrically, and automatically recorded. Although the simple springbalance should be regarded as a semi-continuous method of assessment, it has theadvantage that a complete reaction curve can be obtained from a single specimen.The disadvantage of the spring balance is that one is faced with a compromisebetween accuracy and sensitivity. For accuracy a large specimen is required whereasfor sensitivity one needs to use a relatively fragile spring. It is obviously not possibleto use a fragile spring to carry a large specimen and so the accuracy that is obtainedby this method is a matter of compromise between these two factors. By far the most popular, most convenient, and, unfortunately, most expensivemethod of assessing oxidation reactions is to use the continuous automatic record-ing balance. Obviously the operator must decide precisely what is needed in termsof accuracy and sensitivity from the balance. For straightforward oxidation experi-ments it is generally adequate to choose a balance with a load-carrying ability of upto about 25 g and an ultimate sensitivity of about 100 µg. This is not a particularlysensitive balance and it is rather surprising that many investigators use far moresophisticated, and expensive, semi-micro balances for this sort of work. In factmany problems arise from the use of very sensitive balances together with smallspecimens, to achieve high accuracy. This technique is subject to errors causedby changes in Archimedean buoyancy when the gas composition is changed orthe temperature is altered. An error is also introduced as a result of a change indynamic buoyancy when the gas ﬂow rate over the specimen is altered. For themost trouble-free operation it is advisable to use a large specimen with a large ﬂatsurface area in conjunction with a balance of moderate accuracy. Figure 1.3 showsa schematic diagram of a continuously reading thermobalance used in the authors’laboratory. Using the automatic recording balance it is possible to get a continuous recordof the reaction kinetics and, in this way, many details come to light that are hiddenby other methods. For instance spalling of small amounts of the oxide layer isimmediately detected as the balance registers the mass loss; separation of the scalefrom the metal surface is recorded when the balance shows a slow reduction in ratewell below rates that would be expected from the normal reaction laws; cracking ofthe scale is indicated by immediate small increases in the rate of mass gain. Thesefeatures are shown in Figure 1.4. The correct interpretation of data yielded by theautomatic recording balance requires skill and patience but, in almost every case,is well worthwhile. Gas consumptionContinuous assessment based on measurement of the consumption of gas may bedone in two ways. If the system is held at constant volume then the fall in pressuremay be monitored, continuously or discontinuously. Unfortunately, allowing the
Measurements of reaction kinetics 7 Protective casing Automatic recording balance Balance shield gas inlet Balance shield gas exit Specimen Narrow-bore counterweight pyrex tube Reaction chamber gas exit Silica or Pt suspension fiber Silica or refractory tube with ground joint Specimen Reaction chamber gas inlet Tube furnace Thermocouple Figure 1.3 Typical experimental arrangement for measuring oxidation kinetics with an automatic recording balance.pressure of the oxidant to vary appreciably during the reaction is almost certain tocause changes in the rate at which the reaction proceeds. The second method is tomaintain the apparatus at constant pressure and to measure the fall in volume asoxidizing gas is consumed; this can be done automatically and the results plottedusing a chart recorder. This technique is only useful when the atmosphere is a puregas, for instance pure oxygen. In the case of a mixture of gases such as air, the fallin volume would represent the amount of oxygen consumed but, since nitrogen isnot being consumed, the partial pressure of oxygen would fall, leading to possiblechanges in oxidation rate. This problem can, to some extent, be overcome by using avery large volume of gas compared with the amount of gas used during the reaction.In this case there remains the difﬁculty of measuring a small change in a large
8 Methods of investigation Recorded curve Some scale spalls Weight gain Parabolic extrapolation Scale cracks of initial results Metal-scale separation begins Time Figure 1.4 Hypothetical mass-gain versus time curve for an oxidation reac- tion showing exaggerated, possible features that would be revealed by continu- ous monitoring but missed by a discontinuous technique – leading to erroneous interpretation.volume. Other difﬁculties associated with the measurement of gas consumptionarise from the sensitivity of these methods to variations in room temperature andatmospheric pressure. Accelerated life testsIn some cases a measure of the reaction kinetics is not as useful as a measure ofthe useful life under a given set of experimental conditions. Cyclic oxidation testsusing weight-change versus time measurements and visual examination of exposedspecimens can be useful to determine times beyond which protective scales, suchas alumina, are no longer formed on alloy test coupons. In the case of alloys used in electric heaters the useful life of an alloy is determined(American Society for Testing of Materials, ASTM, B76) by electrically heatinga section of wire in air to a given temperature where it is held for two minutesfollowed by two minutes of cooling. This cycle is repeated until a 10% increase inelectrical resistivity is noted and the time is reported as the useful life of the alloy. Methods of specimen examinationThe oxidation morphology may be examined by a wide range of techniques depend-ing on the particular type of information being sought. The following procedure
Methods of specimen examination 9is recommended in most instances. Initially, the specimen should be examined bythe naked eye and under a low-power binocular microscope, note being taken ofwhether the scale surface is ﬂat, rippled, contains nodules, is cracked, or whetherthere is excessive attack on the edges or in the centers of the faces. This typeof examination is important because subsequent examination generally involvesmicroscopy of a section at a speciﬁc place and it is important to know whetherthis is typical or if there are variations over the specimen surface. It is often worth-while examining the surface in the scanning electron microscope, before sectioning,and, as with all examination, if an area is seen that has signiﬁcant features, pho-tographs must be taken immediately. It is usually too late if one waits for a betteropportunity. In addition, modern scanning electron microscopes allow the chemicalcomposition of surface features to be determined. These techniques are describedbelow. Having examined the scale, it is generally useful to perform X-ray diffraction(XRD) on it to obtain information on the phases present. Studies using XRD canalso provide auxiliary information such as the mechanical stress state in the scale,texture, etc. Preparation of cross-section specimensOnce all the required information on the surface features has been obtained, it isgenerally useful to examine a cross-section of the specimen. This allows observationof the scale thickness and microstructure and any changes that have been producedin the underlying substrate. MountingMetallographic examination involves polishing of a section and, under the polishingstresses, the scale is likely to fall away from the specimen. The specimen with itssurrounding scale must, therefore, be mounted. By far the best type of mountingmedium has been found to be the liquid epoxy resins. The process is very easy – adish is greased, the specimen is positioned and the resin is poured in. At this stagethe dish should be evacuated in a dessicator, left under vacuum for a few minutes,and then atmospheric pressure reapplied. This has the effect of removing air fromcrevices caused by cracks in the scale and on reapplying pressure the resin is forcedinto cavities left by evacuation. This sort of mounting procedure requires severalhours for hardening, preferably being left in a warm place overnight, but the goodsupport which is given to the fragile scales is well worth the extra time and effort.When emphasis must be placed on edge retention, it may be necessary to backupthe specimen with metal shims prior to the mounting operation.
10 Methods of investigation PolishingIt is important at this stage to realize that polishing is carried out for the oxides andnot for the metal. A normal metallurgical polish will not reveal the full features ofthe oxide. Normally a metal is polished using successive grades of abrasive paper –the time spent on each paper being equivalent to the time required to remove thescratches left by the previous paper. If this procedure is carried out it will almostcertainly produce scales which are highly porous. It is important to realize that,because of their friability, scales are damaged to a greater depth than that repre-sented by the scratches on the metal, and, when going to a less abrasive paper, itis important to polish for correspondingly longer times in order to undercut thedepth of damage caused by the previous abrasive paper. In other words, polishingshould be carried out for much longer times on each paper than would be expectedfrom examination of the metal surface. If this procedure is carried out, scales whichare nicely compact and free from induced porosity will be revealed. The polishedspecimens may be examined using conventional optical metallography or scanningelectron microscopy (SEM). EtchingFinally, it may be found necessary to etch a specimen to reveal detail in either themetal or the oxide scale. This is done following standard metallographic preparationprocedure with the exception that thorough and lengthy rinsing in a neutral solvent(alcohol) must be carried out. This is necessary because of existence of pores andcracks in the oxide, especially at the scale–metal interface, that retain the etchantby capillary action. Thus extensive soaking in rinse baths is advisable, followedby rapid drying under a hot air stream, if subsequent oozing and staining is to beavoided. Description of specialized examination techniquesIt is assumed that the reader is familiar with the techniques of optical microscopy.There are, however, a number of other specialized techniques, which are useful forexamining various features of oxidation morphologies. These techniques mainlygenerate information from interactions between the specimen and an incident beamof electrons, photons, or ions. The basis for the various techniques will be describedhere. Examples of their application will be presented in subsequent chapters. Figure 1.5 is a schematic diagram of some of the important interactions between asolid specimen and an incident beam of electrons. The incident beam, if sufﬁcientlyenergetic, can knock electrons from inner shells in the atoms in the solid givingrise to characteristic X-rays from each of the elements present as higher-energy
Description of specialized examination techniques 11 Incident electron Characteristic beam X–rays Backscattered electrons Auger electrons Secondary electrons Inelastically Diffracted scattered electrons electrons Transmitted electrons Figure 1.5 Schematic diagram of the interactions of an incident electron beam with a solid specimen.electrons fall into the empty states. Some of the electrons will be elastically scat-tered in the backward direction with the number of backscattered electrons, whichexit the specimen increasing as the average atomic mass of the solid increasesand as the local inclination of the specimen, with respect to the incident beam,increases. Secondary electrons are the result of inelastic scattering of electrons inthe conduction band of the solid, by incident or backscattered electrons, whichgives them enough energy to exit the solid. Auger electrons are ejected from thesolid by a process similar to that which generates characteristic X-rays, i.e., whena higher-energy electron falls into a vacated state, the energy released results inthe ejection of an electron from an outer shell rather than creation of an X-ray. Ifthe specimen is thin enough, some of the electrons will pass through the specimen.These will comprise a transmitted beam, which will contain electrons from theincident beam that have not undergone interactions or have lost energy as the resultof inelastic scattering processes, and a diffracted beam of electrons, which havesatisﬁed particular angular relations with lattice planes in the solid. Figure 1.6 is a schematic diagram of some of the important interactions betweena solid specimen and an incident X-ray beam. These will result in diffractedX-rays, which have satisﬁed particular angular relations with lattice planes in thesolid and will, therefore, contain crystallographic information. The interactionswill also result in the ejection of photoelectrons, which will have energies equal tothe difference between that of the incident photon and the binding energy of theelectron in the state from which it is ejected.
12 Methods of investigation Figure 1.6 Schematic diagram of the interactions of an incident X-ray beam with a solid specimen. The following is a brief description of the electron-optical and other specializedtechniques, which may be used for examining oxidation morphologies, and thetype of information which may be obtained from each technique. The reader isdirected to the texts and reviews, referenced for each technique, for a more detaileddescription. Scanning electron microscopy (SEM)Scanning electron microscopy is currently the most widely used tool for charac-terising oxidation morphologies. In this technique2,3 an incident electron beam israstered over the specimen surface while the secondary electrons or backscatteredelectrons enter a detector creating an electrical signal which is used to modulatethe intensity of a TV monitor, which is being rastered at the same rate as theelectron beam. This produces an image which indicates the topography of the spec-imen, since the number of secondary or backscattered electrons which escape thespecimen will depend on the local tilt of the specimen surface, and does so withgreat depth of focus. Also, information regarding the average atomic mass can beobtained if the image is formed using backscattered electrons. Modern scanningelectron micrographs,3 equipped with ﬁeld-emission electron guns, can achievemagniﬁcations as high as 100 000 × and resolutions of 1000 nm. Since the incident electrons also produce characteristic X-rays from the elementsin the solid, information can be obtained with regard to the elements present and,if suitable corrections are made, their concentration. The output from the X-ray
Description of specialized examination techniques 13detector can also be used to modulate the intensity of the monitor, which allows amap of the relative concentration of a given element to be produced. The ability toprovide information with regard to microstructure and composition, simultaneously,makes SEM an extremely valuable tool in studying oxidation morphologies. X-ray diffraction (XRD)In this technique the specimen is bombarded with a focused beam of monochro-matic X-rays.4 The beam will be diffracted by the lattice planes, which satisfyBragg’s law, Equation (1.2), where λ is the wavelength of the X-rays, dhkl is nλ = 2dhkl sin θ (1.2)the interplanar spacing of the lattice plane, θ is the angle between the incident beamand the lattice plane, and n is the order of the reﬂection. Determination of the angles at which diffraction occurs allows determinationof the spacing of the various lattice planes and, therefore, the crystal structure ofthe phase or phases present in the solid. Comparison of the d values with tab-ulated values for various substances can be used to identify the phases presentin the specimen. This has resulted in XRD being used for many years to iden-tify the phases present in oxide layers formed on metals and alloys. Modern X-raydiffractometers, with glancing-angle capabilities, can analyze oxide layers as thin as1000 nm. An additional useful feature of XRD is that the positions of the diffraction peaksshift if the solid is strained. Use of specialized diffraction techniques5 allow thesestrains to be measured, which then allows determination of the state of stress in theoxide layer and, in some cases, the underlying metal substrate. Transmission electron microscopy (TEM)When higher spatial resolution examination of specimens is needed, transmissionelectron microscopy (TEM) is utilized.3,6 Here a specimen thin enough to transmitthe electron beam is required. This can be achieved by thinning the specimendirectly or mounting it and thinning a cross-section.7 If small precipitates are thefeature of interest, they can sometimes be examined by preparing carbon extractionreplicas from the specimen. Figure 1.5 indicates that electrons, which have undergone several types of inter-action with the specimen, exit the bottom side. The transmitted beam has passedthrough the specimen with essentially no interaction. The diffracted beams con-tain electrons, which have not lost energy (elastically scattered) but have satisﬁedangular criteria (similar to Bragg’s law for X-rays) and have been scattered intoa new path. The transmitted and diffracted beams can be used to form images ofthe specimen with very high resolution (on the order of 1 nm). Additionally the
14 Methods of investigationdiffracted electrons can be used to form a selected area diffraction (SAD) patternfrom a small region of the specimen, which yields crystallographic information ina manner analogous to XRD patterns. Electrons which have lost energy by interaction with the specimen (inelasticallyscattered electrons) also exit the specimen. The amounts of energy lost by theelectrons can be measured and form the basis for several types of electron energy-loss spectroscopies (EELS) which allow high-resolution chemical analysis to beperformed. Finally, characteristic X-rays are also produced in TEM, as they are in SEM,and can be analyzed to yield chemical-composition information. The X-rays aregenerated in a smaller specimen volume in TEM than SEM and, therefore, smallerfeatures can be analyzed. Surface analytical techniquesIn many cases it is of interest to have information about compositions in very thinlayers of materials, such as the ﬁrst-formed oxide on an alloy. A group of techniques,which are highly surface sensitive, are available for such determinations.8 Grabkeet al.9 have presented a good review of the application of these techniques in theanalysis of oxidation problems. The most widely used technique is Auger electron spectroscopy (AES). Sincethe Auger electrons are emitted as the result of transitions between electron levels,their energies are element speciﬁc and all elements, with the exception of H andHe, can be detected.9 Also, since the energies of Auger electrons are low (20eV–2.5 keV) they are only emitted from shallow depths, of a few atomic layers,giving the technique its surface sensitivity. Auger spectra can be quantiﬁed usingstandards and published correction factors, and if the incident beam is scanned overthe specimen surface, can be used to generate composition maps analogous to theX-ray maps from a scanning electron micrograph. The incident electron beam inmodern instruments can be focussed to give analyses with lateral spatial resolutionon the order of 50 nm.9 The photoelectrons produced by bombarding the specimens with X-rays can alsobe used to obtain chemical information in a technique called X-ray photoelectronspectroscopy (XPS). Photoelectrons have energies similar to Auger electrons sothe specimen depth analyzed is similar to that in AES. However, since it is difﬁcultto bring an X-ray beam to a ﬁne focus the spatial resolution is poorer than thatachievable in AES. An advantage of XPS is that, since the photoelectron energy isa function of the binding energy of the electron in the solid, it can give informationregarding the ionization state of an element, i.e., whether it is present in elementalform, as an oxide, as a nitride, etc.
References 15 Secondary-ion mass spectroscopy (SIMS) is another useful technique, whichinvolves sputtering away the surface of the specimen with an ion beam and analyzingthe sputtered ions in a mass spectrometer. The SIMS technique can provide veryprecise chemical analysis of very thin surface layers and, as sputtering proceeds, aconcentration–depth proﬁle through the specimen. The application of the above techniques is an important part of the study ofoxidation, so much so that regular conferences are now held on this subject.10–14It is important to emphasize that proper investigation of oxidation mechanismsinvolves as many of the above techniques of observing kinetics and morphologiesas feasible, and careful combination of the results. References 1. S. Mrowec and A. J. Stoklosa, J. Therm. Anal., 2 (1970), 73. 2. J. I. Goldstein, D. E. Newbury, P. Echlin, et al., Scanning Electron Microscopy and X-Ray Microanalysis, New York, NY, Plenum Press, 1984. 3. M. H. Loretto, Electron Beam Analysis of Materials, 2nd edn., London, UK, Chapman and Hall, 1994. 4. B. D. Cullity, Elements of X-Ray Diffraction, 2nd edn, Reading, MA, Addison Wesley, 1978. 5. I. C. Noyan and J. B. Cohen, Residual Stresses, New York, NY, Springer-Verlag, 1987. 6. D. B. Williams and C. B. Carter, Transmission Electron Microscopy, New York, NY, Plenum Press, 1996. 7. M. R¨ hle, U. Salzberger and E. Schumann. High resolution transmission microscopy u of metal/metal oxide interfaces. In Microscopy of Oxidation 2, eds. S. B. Newcomb and M. J. Bennett, London, UK, The Institute of Materials, 1993, p. 3. 8. D. P. Woodruff and T. A. Delchar, Modern Techniques of Surface Science, Cambridge, UK, Cambridge University Press, 1989. 9. H. J. Grabke, V. Leroy and H. Viefhaus, ISIJ Int., 35 (1995), 95.10. Microscopy of Oxidation 1, eds. M. J. Bennett and G. W. Lorimer, London, UK, The Institute of Metals, 1991.11. Microscopy of Oxidation 2, eds. S. B. Newcomb and M. J. Bennett, London, UK, The Institute of Materials, 1993.12. Microscopy of Oxidation 3, eds. S. B. Newcomb and J. A. Little, London, UK, The Institute of Materials, 1997.13. Microscopy of Oxidation 4, eds. G. Tatlock and S. B. Newcomb, Science Rev., 17 (2000), 1.14. Microscopy of Oxidation 5, eds. G. Tatlock and S. B. Newcomb, Science Rev., 20 (2003).
2 Thermodynamic fundamentals IntroductionA sound understanding of high-temperature corrosion reactions requires the deter-mination of whether or not a given component in a metal or alloy can react with agiven component from the gas phase or another condensed phase, and to rationalizeobserved products of the reactions. In practice, the corrosion problems to be solvedare often complex, involving the reaction of multicomponent alloys with gases con-taining two or more reactive components. The situation is often complicated by thepresence of liquid or solid deposits, which form either by condensation from thevapour or impaction of particulate matter. An important tool in the analysis of suchproblems is, of course, equilibrium thermodynamics which, although not predic-tive, allows one to ascertain which reaction products are possible, whether or notsigniﬁcant evaporation or condensation of a given species is possible, the conditionsunder which a given reaction product can react with a condensed deposit, etc. Thecomplexity of the corrosion phenomena usually dictates that the thermodynamicanalysis be represented in graphical form. The purpose of this chapter is to review the thermodynamic concepts pertinentto gas–metal reactions and then to describe the construction of the thermodynamicdiagrams most often used in corrosion research, and to present illustrative examplesof their application. The types of diagrams discussed are(1) Gibbs free energy versus composition diagrams and activity versus composition dia- grams, which are used for describing the thermodynamics of solutions.(2) Standard free energy of formation versus temperature diagrams which allow the ther- modynamic data for a given class of compounds, oxides, sulphides, carbides, etc., to be presented in a compact form.(3) Vapour-species diagrams which allow the vapour pressures of compounds to be presented as a function of convenient variables such as partial pressure of a gaseous component. 16
Basic thermodynamics 17(4) Two-dimensional, isothermal stability diagrams, which map the stable phases in systems involving one metallic and two reactive, non-metallic components.(5) Two-dimensional, isothermal stability diagrams which map the stable phases in systems involving two metallic components and one reactive, non-metallic component.(6) Three-dimensional, isothermal stability diagrams which map the stable phases in sys- tems involving two metallic and two reactive, non-metallic components. Basic thermodynamicsThe question of whether or not a reaction can occur is answered by the second law ofthermodynamics. Since the conditions most often encountered in high-temperaturereactions are constant temperature and pressure, the second law is most convenientlywritten in terms of the Gibbs free energy (G ) of a system, Equation (2.1), G = H −TS , (2.1)where H is the enthalpy and S the entropy of the system. Under these conditionsthe second law states that the free-energy change of a process will have the follow-ing signiﬁcance: G < 0, spontaneous reaction expected; G = 0, equilibrium; G > 0, thermodynamically impossible process. For a chemical reaction, e.g. Equation (2.2), aA + bB = cC + dD, (2.2) G is expressed as in Equation (2.3), c d aC aD G = G ◦ + RT ln a b , (2.3) aA aBwhere G ◦ is the free-energy change when all species are present in their standardstates; a is the thermodynamic activity, which describes the deviation from thestandard state for a given species and may be expressed for a given species i as inEquation (2.4), pi ai = ◦ . (2.4) piHere pi is either the vapour pressure over a condensed species or the partial pressureof a gaseous species and pi◦ is the same quantity corresponding to the standard stateof i. Expressing ai by Equation (2.4) requires the reasonable approximation ofideal gas behaviour at the high temperatures and relatively low pressures usuallyencountered. The standard free-energy change is expressed for a reaction such asEquation (2.2) by Equation (2.5), G◦ = c G◦ + d G◦ − a G◦ − b G◦ , C D A B (2.5)
18 Thermodynamic fundamentalswhere G ◦ , etc., are standard molar free energies of formation which may be Cobtained from tabulated values. (A selected list of references for thermodynamicdata such as G ◦ is included at the end of this chapter.) For the special cases ofequilibrium ( G = 0) Equation (2.3) reduces to Equation (2.6), c d aC aD G ◦ = −RT ln a b . (2.6) aA aB eqThe term in parentheses is called the equilibrium constant (K) and is used to describethe equilibrium state of the reaction system. Construction and use of thermodynamic diagrams (a) Gibbs free energy versus composition diagrams and activity versus composition diagramsThe equilibrium state of a system at constant temperature and pressure is charac-terized by a minimum in the Gibbs free energy of the system. For a multicom-ponent, multiphase system, the minimum free energy corresponds to uniformityof the chemical potential (µ) of each component throughout the system. For abinary system, the molar free energy (G) and chemical potentials are related byEquation (2.7), G = (1 − X )µA + X µB , (2.7)where µA and µB are the chemical potentials of components A and B, respectively,and (l − X) and X are the mole fractions of A and B. Figure 2.1(a) is a plot of Gversus composition for a single phase which exhibits simple solution behaviour. Itcan readily be shown,1,2 starting with Equation (2.7), that for a given compositionµA and µB can be deﬁned as in Equations (2.8) and (2.9), dG µA = G − X ; (2.8) dX dG µB = G + (1 − X ) , (2.9) dXwhich, as indicated in Figure 2.1(a), means that a tangent drawn to the free-energycurve has intercepts on the ordinate at X = 0 and X = 1, corresponding to thechemical potentials of A and B, respectively. Alternatively, if the free energy ofthe unmixed components in their standard states, (1 − X )µ◦ + X µ◦ is subtracted A Bfrom each side of Equation (2.7), the result is the molar free energy of mixing,Equation (2.10): G M = (1 − X )(µA − µ◦ ) + X (µB − µ◦ ). A B (2.10)
Construction and use of thermodynamic diagrams 19 Gβ µB Gα← ←G G G µB dG (1 −X ) ––– dXµA µA α α+β β A B A X1 X2 B ← X X ← (a) (b) Figure 2.1 Free energy versus composition diagrams for (a) one phase, and (b) two coexisting phases.A plot of G M versus X may be constructed in which case the tangent interceptsare (µA − µ◦ ) and (µB − µ◦ ), respectively. These quantities, the partial molar free A Benergies of mixing, are directly related to the activities of the given componentthrough Equations (2.11) and (2.12): µA − µ◦ = RT ln aA , A (2.11) µB − µ◦ = RT ln aB . B (2.12) Figure 2.1(b) shows the free energy versus composition diagram for two phases.Application of the lever rule shows that the free energy for a mixture of the twophases is given by the point where the chord, drawn between the two individual free-energy curves, intersects the bulk composition. Clearly, for any bulk compositionbetween X1 and X2 in Figure 2.1(b), a two-phase mixture will have a lower freeenergy than a single solution corresponding to either phase, and the lowest freeenergy of the system, i.e., the lowest chord, results when the chord is in fact atangent to both free-energy curves. This ‘common-tangent construction’ indicatesX1 and X2 to be the equilibrium compositions of the two coexisting phases and theintercepts of the tangent at X = 0 and X = 1 show the construction is equivalentto the equality of chemical potentials, i.e., Equations (2.13) and (2.14): β µ α = µA , A (2.13) β µ α = µB . B (2.14)
20 Thermodynamic fundamentals a*← ← a* a)a a a) X* ← X* ← = Figure 2.2 Activity versus composition diagrams for a solution exhibiting (a) positive- and (b) negative-deviation from Raoult’s law. Equations 2.11 and 2.12 indicate that similar information may be expressed interms of activity. Figure 2.2 shows activity versus composition plots for a sys-tem with a free-energy curve such as that in Figure 2.1(a); with Figure 2.2(a)corresponding to a slightly positive deviation from Raoult’s law (a X) andFigure 2.2(b) corresponding to a slightly negative deviation (a X). For caseswhere a two-phase mixture is stable, Figure 2.1(b), Equations (2.13) and (2.14)indicate the activities are constant across the two-phase ﬁeld. Figure 2.3 illustratesthe above points and their relationship to the conventional phase diagram for ahypothetical binary eutectic system. For a comprehensive treatment of free-energydiagrams and their applications to phase transformations the reader is referred tothe excellent article by Hillert.3 Clearly, if the variation of G or G M with composition for a system can beestablished, either by experimental activity measurements or by calculations usingsolution models, the phase equilibria can be predicted for a given temperatureand composition. Considerable effort has been spent in recent years on computercalculations of phase diagrams, particularly for refractory metal systems (see forexample ref. 4). Furthermore, the concepts need not be limited to binary elemen-tal systems. For example, ternary free-energy behaviour may be described on athree-dimensional plot, the base of which is a Gibbs triangle and the vertical axisrepresents G (or G M ). In this case, the equilibrium state of the system is describedusing a ‘common tangent plane’, rather than a common tangent line, but the princi-ples are unchanged. Systems with more than three components may be treated, butgraphical interpretation becomes more difﬁcult. Also, the above concepts may be
Construction and use of thermodynamic diagrams 21 (l) (l) (l) ← T T1 α β T α β α β 2 T3 α α β β (l) α (l) β ← (l) G aA aB aB ← aA aB aA a A XB ← B A XB ← B A XB ← B Figure 2.3 Free energy versus composition and activity diagrams for a hypothetical eutectic system.applied to pseudo-binary systems where the components are taken as compoundsof ﬁxed stoichiometry. Figure 2.4 shows the activity versus composition plot5 forsuch a system, Fe2 O3 –Mn2 O3 . This type of diagram may be constructed for anyof the systems encountered in high-temperature corrosion, e.g., sulphides, oxides,sulphates, etc., and is useful in interpreting corrosion products and deposits formedon metallic or ceramic components.
22 Thermodynamic fundamentals 1.0 0.8 0.6 a MnO1.5 a FeO1.5 a→ 0.4 0.2 Fe2O3 0.2 0.4 0.6 0.8 Mn2O3 X MnO1.5→ Figure 2.4 Activity versus composition diagram for the Fe2 O3 –Mn2 O3 system at 1300 ◦ C (see ref. 5). (b) Standard free-energy-of-formation versus temperature diagramsOften determination of the conditions under which a given corrosion product islikely to form is required, e.g., in selective oxidation of alloys. In this regard,Ellingham diagrams, i.e., plots of the standard free energy of formation ( G ◦ )versus temperature for the compounds of a type, e.g., oxides, sulphides, carbides,etc., are useful in that they allow comparison of the relative stabilities of eachcompound. Figure 2.5 is such a plot for many simple oxides. The values of G ◦are expressed as kJ mol−1 O2 so the stabilities of various oxides may be compareddirectly, i.e., the lower the position of the line on the diagram the more stable is theoxide. Put another way, for a given reaction, Equation (2.15), M + O2 = MO2 , (2.15)if the activities of M and MO2 are taken as unity, Equation (2.6) may be used toexpress the oxygen partial pressure at which the metal and oxide coexist, i.e., thedissociation pressure of the oxide, Equation (2.16): M/MO2 G◦ p O2 = exp . (2.16) RT
Construction and use of thermodynamic diagrams 23 H2/H2O ratio 10−8 10−6 10−4 pO 2 CO/CO2 ratio −8 −6 −4 −2 10 10 10 10 10−2 0 1O O3 Fe 2 =6 1 −100 +O 2 CO 2 10−2 M =2 O4 C oO + O2 e3 =2 2CO M M 4F O2 1 o+ = 2H 2 O −200 O NiO 2C 2H 2+ 2Cu 2 M O2 = =2 10−4 + O2 + O2 4Cu i 2N −300 102 ∆G ° = RT ln pO2 (KJ mol−1 O2) 10−6 C + O2 = CO2 102 −400 M M O Zn 10−8 =2 B 2CH −500 O2 2 Cr 2 O3 +O 104 n+ =3 2 =2 2Z + O2 O CO 4 Cr NbC =2 10−10 M 3 M −600 b + O2 B 2N 10 4 iO 2 =S −700 O2 10−12 Si + 106 O3 2 Cr 2 −800 = 3 + O2 10−14 4 Cr 3 106 TiO −900 =2 10−16 B + O2 M B 108 2Ti 2 A l 2O 3 −1000 = 3 4 Al + O 2 2MgO M 3 = M Change of state Element Oxide 10−18 O2 −1100 g+ Ca O Melting point M M 108 2M =2 a + O2 Boiling point B B 2C 1010 10−20 −1200 0 200 400 600 800 1000 1200 1400 1600 1800 2000 2200 2400 Temperature (°C) 1010 10−22 CO/CO2 ratio 1014 1012 0K H2/H2O ratio 10−200 10−100 10−70 10−60 10−50 10−42 10−38 10−34 10−30 10 −28 10−26 10−24 pO 2 Figure 2.5 Standard free energy of formation of selected oxides as a function of temperature.Naturally, in considering alloy oxidation, the activity of the metal and oxide mustbe taken into account, i.e., Equation (2.17): eq aMO2 G◦ aMO2 M/MO2 pO2 = exp = p . (2.17) aM RT a M O2
24 Thermodynamic fundamentals M/MOThe values of pO2 2 may be obtained directly from the oxygen nomograph onthe diagram by drawing a straight line from the origin marked O through the free-energy line at the temperature of interest and reading the oxygen partial pressurefrom its intersection with the scale at the right side labelled pO2 . Values for thepressure ratio H2 /H2 O for equilibrium between a given metal and oxide may beobtained by drawing a similar line from the point marked H to the scale labelledH2 /H2 O ratio and values for the equilibrium CO/CO2 ratio may be obtained bydrawing a line from point C to the scale CO/CO2 ratio. The reader is referred toGaskell (ref. 2, Chapter 12), for a more detailed discussion of the construction anduse of Ellingham diagrams for oxides. Ellingham diagrams may, of course, be constructed for any class of compounds.Shatynski has published Ellingham diagrams for sulphides6 and carbides.7 Elling-ham diagrams for nitrides and chlorides are presented in chapter 14 of reference 1. (c) Vapour-species diagramsThe vapour species which form in a given high-temperature corrosion situation oftenhave a strong inﬂuence on the rate of attack, the rate generally being acceleratedwhen volatile corrosion products form. Gulbransen and Jansson8 have shown thatmetal and volatile oxide species are important in the kinetics of high-temperatureoxidation of carbon, silicon, molybdenum, and chromium. Six types of oxidationphenomena were identiﬁed.(1) At low temperature, diffusion of oxygen and metal species through a compact oxide ﬁlm.(2) At moderate and high temperatures, a combination of oxide-ﬁlm formation and oxide volatility.(3) At moderate and high temperatures, the formation of volatile metal and oxide species at the metal–oxide interface and transport through the oxide lattice and mechanically formed cracks in the oxide layer.(4) At moderate and high temperatures, the direct formation of volatile oxide gases.(5) At high temperature, the gaseous diffusion of oxygen through a barrier layer of volatilised oxides.(6) At high temperature, spalling of metal and oxide particles.Sulphidation reactions follow a similar series of kinetic phenomena as has beenobserved for oxidation. Unfortunately, few studies have been made of the basickinetic phenomena involved in sulphidation reactions at high temperature. Simi-larly, the volatile species in sulphate and carbonate systems are important in termsof evaporation/condensation phenomena involving these compounds on alloy orceramic surfaces. Perhaps the best example of this behaviour is the rapid degra-dation of protective scales on many alloys, termed ‘hot corrosion’, which occurswhen Na2 SO4 or other salt condenses on the alloy.
Construction and use of thermodynamic diagrams 25 Table 2.1 Species Log Kp Cr2 O3 (s) 33.95 Cr (g) −8.96 CrO (g) −2.26 CrO2 (g) 4.96 CrO3 (g) 8.64 The diagrams most suited for presentation of vapour-pressure data in oxidesystems are log pMx O y , for a ﬁxed T, versus log pO2 ; and log pMx O y , for a ﬁxed pO2 ,versus 1/T diagrams. The principles of the diagrams will be illustrated for the Cr–Osystem at 1250 K. Only one condensed oxide, Cr2 O3 , is formed under conditionsof high-temperature oxidation. Thermochemical data are available for Cr2 O3 (s),9Cr (g),10 and the three gaseous oxide species CrO (g), CrO2 (g), and CrO3 (g).11These data may be expressed as standard free energies of formation ( G ◦ ), or,more conveniently, as log Kp deﬁned by Equation (2.1): − G◦ log K p = . (2.18) 2.303RT The appropriate data at 1250 K are listed in Table 2.1.The vapour pressures of species in equilibrium with Cr metal must be determinedfor low oxygen pressures and those of species in equilibrium with Cr2 O3 at highoxygen pressures. The boundary between these regions is the oxygen pressure forthe Cr/Cr2 O3 equilibrium, obtained from the equilibrium given in Equation (2.17), 3 2Cr (s) + O2 (g) = Cr2 O3 (s), (2.19) 2for which log p O2 has the value given in Equation (2.20): 2 log pO2 = − log K Cr2 O3 = −22.6. p (2.20) 3The boundary is represented by the vertical line in Figure 2.6. At lower oxygenpressures the pressure of Cr (g) is independent of pO2 : Cr (s) = Cr (g), (2.21) log pCr = log K Cr (g) = −8.96. p (2.22)For oxygen pressures greater than Cr/Cr2 O3 equilibrium, the vapour pressure of Crmay be obtained from Equation (2.23), 3 Cr2 O3 (s) = 2 Cr (g) + O2 (g), (2.23) 2
26 Thermodynamic fundamentals log (p − H2/p − H2O) 14 12 10 8 6 4 2 0 −2 −4 −6 4 0 Cr (s) −4 Cr2O3 (s) log p Crx Oy (atm) −8 Cr (g) −12 −16 (g) CrO (g ) −20 ) 3 (g O O2 Cr Cr −24 −44 −40 −36 −32 −28 −24 −20 −16 −12 −8 −4 0 log p O2(atm) Figure 2.6 Volatile species in the Cr–O system at 1250 K.with the equilibrium constant, K23 , determined from Equation (2.24): log K 23 = 2 log K Cr (g) − log K Cr2 O3 = −51.9. p p (2.24)Therefore, Equations (2.25) or (2.26) are obtained: 3 2 log pCr + log pO2 = −51.9, (2.25) 2 3 log pCr = −25.95 − log pO2 . (2.26) 4The vapour pressure of Cr is then expressed in Figure 2.6 by plotting Equations(2.22) and (2.26). The lines corresponding to the other vapour species are obtainedin the same manner. For example, for CrO3 at oxygen pressures below Cr/Cr2 O3equilibrium we have Equations (2.27) and (2.28): 3 Cr (s) + O2 (g) = CrO3 (g), (2.27) 2 log K 27 = log K CrO3 (g) = 8.64, p (2.28)from which one ﬁnds log pCrO3 , Equation (2.29): 3 log pCrO3 = 8.64 + log pO2 . (2.29) 2
Construction and use of thermodynamic diagrams 27 T (K) 1150 1200 1250 1300 1342 1400 1450 0 −2 Mixed −4 oxidation and volatilitylog pCrx Oy (atm) −6 O Enhanced CrO3 (g) Cr2O3 (s)/ 2 oxidation ) −8 (s)/Cr (s due to Cr Cr 2O 3 vapour Normal −10 oxidation Cr (g) −12 −14 0.88 0.86 0.84 0.82 0.80 0.78 0.76 0.74 0.72 0.70 0.68 1/T × 103 (K−1) Figure 2.7 Cr–O system volatile species versus temperature. The line for Cr (g) refers to the pressure at the Cr–Cr2 O3 interface and the CrO3 (g) line refers to the Cr2 O3 /gas interface for an oxygen partial pressure of 1 atm. The other lines in Figure 2.6 are obtained by writing similar equilibrium equa- tions. Figure 2.6 shows that signiﬁcant vapour pressures of Cr are developed at low pO2 , e.g., at the alloy–scale interface of a Cr2 O3 -forming alloy, and that very large pressures of CrO3 are developed at high pO2 . The latter are responsible for a phenomenon whereby Cr2 O3 scales are thinned by vapour losses during oxidation at high pO2 , particularly for high gas ﬂow rates. Figure 2.7 indicates the tempera- ture dependence of the various equilibria. Similar diagrams may be constructed for other oxides, sulphides, halides, etc. (d) Two-dimensional, isothermal stability diagram: one metallic and two non-metallic components When a metal reacts with a gas containing more than one oxidant, a number of different phases may form depending on both thermodynamic and kinetic consid- erations. Isothermal stability diagrams, usually constructed with the logarithmic values of the activities or partial pressures of the two non-metallic components as
28 Thermodynamic fundamentals Table 2.2 Species log Kp NiO (s) 5.34 NiSy (l) 3.435 NiSO4 (s) 15.97 SO2 (g) 11.314 SO3 (g) 10.563 S (l) −0.869the coordinate axes, are useful in interpreting the condensed phases which form.To illustrate the construction of this type of diagram, the Ni–S–O system at 1250 Kwill be considered. The appropriate data11 are given in Table 2.2. The coordinates chosen to express the equilibria are log pS2 versus log pO2 .(Only one sulphide is considered for simplicity.) The assumption is made that all the condensed species are at unit activity. Thisassumption places important limitations on the use of the diagrams for alloy sys-tems as will be discussed in later sections. Consider ﬁrst the Ni–NiO equilibrium,Equation (2.30), 1 Ni (s) + O2 (g) = NiO (s), (2.30) 2and log pO2 , deﬁned in Equation (2.31), log pO2 = −2 log K NiO = −10.68, p (2.31)resulting in the vertical phase boundary in Figure 2.8. Similarly, for NiSy (1) (y ≈ 1)we have Equations (2.32) and (2.33): y Ni (s) + S2 (g) = NiS y (l), (2.32) 2 log pS2 = −6.87, (2.33)resulting in the horizontal boundary in Figure 2.8. Equations (2.31) and (2.33),therefore, deﬁne the gaseous conditions over which metallic Ni is stable. In asimilar manner, the other phase boundaries are determined. For example, for theNiO–NiSO4 equilibrium represented by Equations (2.34) and (2.35). 1 3 NiO (s) + S2 (g) + O2 (g) = NiSO4 (s), (2.34) 2 2 log K 34 = log K NiSO4 − log K NiO = 10.63, p p (2.35)resulting in Equation (2.36) for the phase boundary: log pS2 = −21.26 − 3 log pO2 . (2.36)